Ferromagnetic Order from p-Electrons in Rubidium Oxide
Riyadi, Syarif; Giriyapura, Shivakumara; de Groot, Robert A.; Caretta, Antonio; van Loosdrecht, Paul H. M.; Palstra, Thomas T. M.; Blake, Graeme R.; Chemistry of Materials 23 (2011) 1578–; doi:10.1021/cm103433r

data_4000747
_publ_section_title
;
 Ferromagnetic Order from p-Electrons in Rubidium Oxide
;
_journal_issue                   6
_journal_name_full               'Chemistry of Materials'
_journal_page_first              1578
_journal_paper_doi               10.1021/cm103433r
_journal_volume                  23
_journal_year                    2011
_chemical_formula_sum            'O6.88 Rb4'
_chemical_formula_weight         451.95
_chemical_name_systematic        ' ?'
_space_group_IT_number           69
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-F 2 2'
_symmetry_space_group_name_H-M   'F m m m'
_audit_creation_date             2010-12-01T11:01
_audit_creation_method           'from EXP file using GSAS2CIF'
_audit_update_record
' 2010-12-01T11:01  Initial CIF as created by GSAS2CIF'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                90.0
_cell_formula_units_Z            1
_cell_length_a                   6.30280(29)
_cell_length_b                   6.25587(23)
_cell_length_c                   5.81797(7)
_cell_measurement_temperature    20
_cell_volume                     229.400(14)
_computing_structure_refinement  GSAS
_diffrn_ambient_temperature      20
_diffrn_radiation_polarisn_ratio 0.7
_diffrn_radiation_probe          x-ray
_diffrn_radiation_wavelength     1.54059
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  1.00000
_exptl_absorpt_process_details
;   GSAS Absorption/surface roughness correction: function number 4
 Flat plate transmission absorption correction
Terms =      0.0000         0.0000    
Correction is not refined.
;
_pd_block_id                     2010-12-01T11:01|RBO2-D_20K|graeme|D8
_pd_calc_method                  'Rietveld Refinement'
_pd_char_colour                  yellow
_pd_instr_location               ' ?'
_pd_meas_2theta_range_inc        0.005
_pd_meas_2theta_range_max        70.0
_pd_meas_2theta_range_min        10.01
_pd_meas_number_of_points        11999
_pd_phase_name                   RbO2_lowT
_pd_proc_2theta_range_inc        0.005
_pd_proc_2theta_range_max        71.3375
_pd_proc_2theta_range_min        11.3475
_pd_proc_info_datetime           2010-12-01T11:01:08
_pd_proc_info_excluded_regions   ' ?'
_pd_proc_ls_background_function
;   GSAS Background function number 1 with 12 terms.
 Shifted Chebyshev function of 1st kind
      1:    505.106     2:    6.02265     3:   -10.7949     4:    5.24962    
      5:    1.92834     6:    4.40346     7:   0.684686     8:   -2.09726    
      9:   0.559522    10:    2.20724    11:   -2.70845    12:   5.564340E-02
;
_pd_proc_ls_peak_cutoff          0.00100
_pd_proc_ls_profile_function
;
 CW Profile function number 4 with  18 terms
 Pseudovoigt profile coefficients as parameterized in
 P. Thompson, D.E. Cox & J.B. Hastings (1987). J. Appl. Cryst.,20,79-83.
 Asymmetry correction of L.W. Finger, D.E. Cox & A. P. Jephcoat (1994).
 J. Appl. Cryst.,27,892-900.
 Microstrain broadening by P.W. Stephens,  (1999). J. Appl. Cryst.,32,281-289.
 Peak tails are ignored  where the intensity is below 0.0010 times the peak
   Aniso. broadening axis   1.0   1.0   0.0
;
_pd_proc_ls_prof_R_factor        0.0101
_pd_proc_ls_prof_wR_expected     0.0431
_pd_proc_ls_prof_wR_factor       0.0143
_pd_proc_number_of_points        11999
_pd_spec_mounting                ' ?'
_refine_ls_goodness_of_fit_all   0.33
_refine_ls_matrix_type           full
_refine_ls_number_parameters     27
_refine_ls_number_restraints     1
_refine_ls_R_Fsqd_factor         0.03820
_refine_ls_shift/su_max          0.06
_refine_ls_shift/su_mean         0.01
_reflns_d_resolution_high        1.434
_reflns_d_resolution_low         3.530
_reflns_limit_h_max              4
_reflns_limit_h_min              0
_reflns_limit_k_max              4
_reflns_limit_k_min              0
_reflns_limit_l_max              4
_reflns_limit_l_min              0
_reflns_number_total             15
_cod_data_source_file            cm103433r_si_002.cif
_cod_data_source_block           RBO2-D_20K_publ
_cod_depositor_comments
;
The following automatic conversions were performed:

'_geom_bond_publ_flag' value 'N' changed to 'n' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (98
times).

'_geom_angle_publ_flag' value 'N' changed to 'n' according
to /home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary
named 'cif_core.dic' version 2.4.1 from 2010-06-29 (510 times).

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 

 Adding full bibliography for 4000747.cif.
;
_cod_original_cell_volume        229.400(6)
_cod_original_formula_sum        'O6.88 Rb4.00'
_cod_database_code               4000747
_gsas_exptl_extinct_corr_t_min   1.00000
_gsas_exptl_extinct_corr_t_max   1.00000